#------------------------------------------------------------------------------
#$Date: 2021-04-30 11:19:27 +0300 (Fri, 30 Apr 2021) $
#$Revision: 264720 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/23/1562309.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562309
loop_
_publ_author_name
'Li, Na'
'Mu, Bao'
'Cao, Xinyu'
'Huang, Rudan'
_publ_section_title
;
 The structures and properties of the new two-dimensional
 inorganic--organic hybrid materials based on the molybdate chains
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              180
_journal_page_last               186
_journal_paper_doi               10.1016/j.jssc.2014.06.001
_journal_volume                  217
_journal_year                    2014
_chemical_formula_sum            'C16 H20 Mo6 N6 O22 Zn'
_chemical_formula_weight         1289.39
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                105.897(2)
_cell_angle_beta                 91.7150(10)
_cell_angle_gamma                98.7490(10)
_cell_formula_units_Z            1
_cell_length_a                   7.6137(6)
_cell_length_b                   10.0890(9)
_cell_length_c                   10.3272(11)
_cell_measurement_reflns_used    2261
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      28.608
_cell_measurement_theta_min      3.154
_cell_volume                     751.92(12)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.974
_diffrn_measured_fraction_theta_max 0.974
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0240
_diffrn_reflns_av_sigmaI/netI    0.0507
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            3717
_diffrn_reflns_theta_full        25.02
_diffrn_reflns_theta_max         25.02
_diffrn_reflns_theta_min         3.16
_exptl_absorpt_coefficient_mu    3.310
_exptl_absorpt_correction_T_max  0.7331
_exptl_absorpt_correction_T_min  0.5872
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_density_diffrn    2.847
_exptl_crystal_density_meas      0
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             616
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.10
_refine_diff_density_max         1.500
_refine_diff_density_min         -1.204
_refine_diff_density_rms         0.250
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.104
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     232
_refine_ls_number_reflns         2572
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.104
_refine_ls_R_factor_all          0.0581
_refine_ls_R_factor_gt           0.0431
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0719P)²+0.2637P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1107
_refine_ls_wR_factor_ref         0.1243
_reflns_number_gt                2029
_reflns_number_total             2572
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2014-217-180.cif
_cod_data_source_block           4
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Triclinic' was changed to
'triclinic' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               1562309
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.20079(9) 0.30810(8) 0.86272(7) 0.0152(2) Uani 1 1 d . . .
Mo2 Mo 0.49942(8) 0.59082(8) 0.87872(7) 0.0134(2) Uani 1 1 d . . .
Mo3 Mo -0.00049(8) 0.57621(8) 0.86283(7) 0.0155(2) Uani 1 1 d . . .
Zn1 Zn 0.5000 0.5000 0.5000 0.0195(3) Uani 1 2 d S . .
N1 N 0.3909(9) 0.7416(8) 0.4034(7) 0.0259(17) Uani 1 1 d . . .
H1 H 0.4240 0.7028 0.3251 0.031 Uiso 1 1 calc R . .
N2 N 0.4079(9) 0.6938(8) 0.5135(7) 0.0252(17) Uani 1 1 d . . .
N3 N 0.1913(9) 1.0620(8) 0.1465(7) 0.0254(17) Uani 1 1 d . . .
H3 H 0.1642 1.1041 0.0886 0.031 Uiso 1 1 calc R . .
O1 O 0.2471(7) 0.5373(6) 0.8790(5) 0.0175(13) Uani 1 1 d . . .
O2 O 0.4579(7) 0.3768(6) 0.9066(5) 0.0162(12) Uani 1 1 d . . .
O3 O -0.0173(7) 0.3743(6) 0.9118(5) 0.0155(12) Uani 1 1 d . . .
O4 O 0.1882(8) 0.2656(6) 0.6888(6) 0.0243(14) Uani 1 1 d . . .
O5 O 0.2412(7) 0.4086(6) 1.0871(5) 0.0177(13) Uani 1 1 d . . .
O6 O 0.1742(7) 0.1500(6) 0.8983(6) 0.0235(14) Uani 1 1 d . . .
O7 O 0.5154(7) 0.5303(7) 0.7061(5) 0.0220(14) Uani 1 1 d . . .
O8 O 0.4973(7) 0.7641(7) 0.9052(6) 0.0245(14) Uani 1 1 d . . .
O9 O -0.0493(7) 0.4971(7) 0.6938(6) 0.0269(15) Uani 1 1 d . . .
O10 O 0.0738(7) 0.7459(7) 0.8713(6) 0.0277(15) Uani 1 1 d . . .
O11 O 0.2332(8) 0.4021(7) 0.4887(6) 0.0297(15) Uani 1 1 d . . .
H11B H 0.1604 0.4465 0.4616 0.036 Uiso 1 1 d R . .
H11C H 0.2033 0.3860 0.5623 0.036 Uiso 1 1 d R . .
C1 C 0.3450(12) 0.7858(11) 0.6127(9) 0.031(2) Uani 1 1 d . . .
H1A H 0.3434 0.7816 0.7015 0.038 Uiso 1 1 calc R . .
C2 C 0.2821(13) 0.8889(10) 0.5671(9) 0.031(2) Uani 1 1 d . . .
H2 H 0.2295 0.9622 0.6168 0.038 Uiso 1 1 calc R . .
C3 C 0.3142(11) 0.8595(9) 0.4338(9) 0.0220(19) Uani 1 1 d . . .
C4 C 0.2820(11) 0.9571(10) 0.1082(9) 0.027(2) Uani 1 1 d . . .
H4 H 0.3164 0.9305 0.0205 0.032 Uiso 1 1 calc R . .
C5 C 0.3244(12) 0.8884(10) 0.1999(9) 0.025(2) Uani 1 1 d . . .
H5 H 0.3875 0.8145 0.1740 0.031 Uiso 1 1 calc R . .
C6 C 0.2735(11) 0.9287(9) 0.3310(8) 0.0219(19) Uani 1 1 d . . .
C7 C 0.1824(13) 1.0422(10) 0.3662(10) 0.030(2) Uani 1 1 d . . .
H7 H 0.1506 1.0746 0.4541 0.036 Uiso 1 1 calc R . .
C8 C 0.1406(13) 1.1046(10) 0.2723(10) 0.034(2) Uani 1 1 d . . .
H8 H 0.0761 1.1778 0.2950 0.041 Uiso 1 1 calc R . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O6 Mo1 O4 104.6(3) . .
O6 Mo1 O3 103.2(3) . .
O4 Mo1 O3 104.7(3) . .
O6 Mo1 O2 102.5(3) . .
O4 Mo1 O2 101.2(2) . .
O3 Mo1 O2 137.2(2) . .
O6 Mo1 O1 164.0(2) . .
O4 Mo1 O1 91.4(2) . .
O3 Mo1 O1 73.2(2) . .
O2 Mo1 O1 72.7(2) . .
O6 Mo1 O5 87.1(3) . .
O4 Mo1 O5 168.0(3) . .
O3 Mo1 O5 75.0(2) . .
O2 Mo1 O5 72.7(2) . .
O1 Mo1 O5 77.0(2) . .
O8 Mo2 O7 103.6(3) . .
O8 Mo2 O1 96.1(3) . .
O7 Mo2 O1 97.7(2) . .
O8 Mo2 O5 100.8(3) . 2_667
O7 Mo2 O5 90.7(2) . 2_667
O1 Mo2 O5 158.8(2) . 2_667
O8 Mo2 O2 90.0(3) . 2_667
O7 Mo2 O2 161.6(3) . 2_667
O1 Mo2 O2 93.0(2) . 2_667
O5 Mo2 O2 74.4(2) 2_667 2_667
O8 Mo2 O2 161.2(2) . .
O7 Mo2 O2 93.7(3) . .
O1 Mo2 O2 74.0(2) . .
O5 Mo2 O2 86.0(2) 2_667 .
O2 Mo2 O2 74.9(2) 2_667 .
O10 Mo3 O9 103.9(3) . .
O10 Mo3 O5 99.0(3) . 2_567
O9 Mo3 O5 98.0(3) . 2_567
O10 Mo3 O1 92.1(3) . .
O9 Mo3 O1 98.8(2) . .
O5 Mo3 O1 157.0(2) 2_567 .
O10 Mo3 O3 158.7(2) . .
O9 Mo3 O3 93.1(3) . .
O5 Mo3 O3 91.1(2) 2_567 .
O1 Mo3 O3 72.4(2) . .
O10 Mo3 O3 91.3(3) . 2_567
O9 Mo3 O3 164.2(3) . 2_567
O5 Mo3 O3 75.0(2) 2_567 2_567
O1 Mo3 O3 84.8(2) . 2_567
O3 Mo3 O3 73.2(2) . 2_567
O7 Zn1 O7 180.000(1) . 2_666
O7 Zn1 O11 89.5(2) . .
O7 Zn1 O11 90.5(2) 2_666 .
O7 Zn1 O11 90.5(2) . 2_666
O7 Zn1 O11 89.5(2) 2_666 2_666
O11 Zn1 O11 180.0 . 2_666
O7 Zn1 N2 86.2(3) . 2_666
O7 Zn1 N2 93.8(3) 2_666 2_666
O11 Zn1 N2 91.0(3) . 2_666
O11 Zn1 N2 89.0(3) 2_666 2_666
O7 Zn1 N2 93.8(3) . .
O7 Zn1 N2 86.2(3) 2_666 .
O11 Zn1 N2 89.0(3) . .
O11 Zn1 N2 91.0(3) 2_666 .
N2 Zn1 N2 180.000(2) 2_666 .
N2 N1 C3 111.1(7) . .
N2 N1 H1 124.5 . .
C3 N1 H1 124.5 . .
C1 N2 N1 104.7(7) . .
C1 N2 Zn1 133.6(6) . .
N1 N2 Zn1 121.6(6) . .
C4 N3 C8 122.2(8) . .
C4 N3 H3 118.9 . .
C8 N3 H3 118.9 . .
Mo2 O1 Mo3 150.8(3) . .
Mo2 O1 Mo1 106.0(2) . .
Mo3 O1 Mo1 102.3(2) . .
Mo1 O2 Mo2 105.6(2) . 2_667
Mo1 O2 Mo2 104.6(2) . .
Mo2 O2 Mo2 105.1(2) 2_667 .
Mo1 O3 Mo3 106.1(2) . .
Mo1 O3 Mo3 103.8(2) . 2_567
Mo3 O3 Mo3 106.8(2) . 2_567
Mo3 O5 Mo2 155.3(3) 2_567 2_667
Mo3 O5 Mo1 102.6(2) 2_567 .
Mo2 O5 Mo1 101.4(2) 2_667 .
Mo2 O7 Zn1 165.2(4) . .
Zn1 O11 H11B 112.7 . .
Zn1 O11 H11C 112.9 . .
H11B O11 H11C 110.5 . .
N2 C1 C2 111.9(8) . .
N2 C1 H1A 124.1 . .
C2 C1 H1A 124.1 . .
C3 C2 C1 105.3(8) . .
C3 C2 H2 127.4 . .
C1 C2 H2 127.4 . .
C2 C3 N1 107.1(8) . .
C2 C3 C6 130.8(8) . .
N1 C3 C6 122.0(8) . .
N3 C4 C5 119.2(8) . .
N3 C4 H4 120.4 . .
C5 C4 H4 120.4 . .
C4 C5 C6 120.3(9) . .
C4 C5 H5 119.9 . .
C6 C5 H5 119.9 . .
C5 C6 C7 117.8(8) . .
C5 C6 C3 123.0(8) . .
C7 C6 C3 119.2(8) . .
C8 C7 C6 119.8(9) . .
C8 C7 H7 120.1 . .
C6 C7 H7 120.1 . .
N3 C8 C7 120.6(9) . .
N3 C8 H8 119.7 . .
C7 C8 H8 119.7 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O6 1.717(6) .
Mo1 O4 1.724(6) .
Mo1 O3 1.914(5) .
Mo1 O2 1.970(5) .
Mo1 O1 2.244(6) .
Mo1 O5 2.251(5) .
Mo2 O8 1.697(6) .
Mo2 O7 1.733(5) .
Mo2 O1 1.915(5) .
Mo2 O5 1.995(5) 2_667
Mo2 O2 2.157(5) 2_667
Mo2 O2 2.232(6) .
Mo3 O10 1.697(6) .
Mo3 O9 1.711(6) .
Mo3 O5 1.936(5) 2_567
Mo3 O1 1.994(5) .
Mo3 O3 2.216(6) .
Mo3 O3 2.238(5) 2_567
Zn1 O7 2.063(5) .
Zn1 O7 2.063(5) 2_666
Zn1 O11 2.104(6) .
Zn1 O11 2.104(6) 2_666
Zn1 N2 2.147(7) 2_666
Zn1 N2 2.147(7) .
N1 N2 1.361(10) .
N1 C3 1.368(11) .
N1 H1 0.8600 .
N2 C1 1.335(12) .
N3 C4 1.327(12) .
N3 C8 1.340(12) .
N3 H3 0.8600 .
O2 Mo2 2.157(5) 2_667
O3 Mo3 2.238(5) 2_567
O5 Mo3 1.936(5) 2_567
O5 Mo2 1.995(5) 2_667
O11 H11B 0.8501 .
O11 H11C 0.8500 .
C1 C2 1.393(13) .
C1 H1A 0.9300 .
C2 C3 1.364(12) .
C2 H2 0.9300 .
C3 C6 1.470(12) .
C4 C5 1.376(12) .
C4 H4 0.9300 .
C5 C6 1.388(12) .
C5 H5 0.9300 .
C6 C7 1.398(13) .
C7 C8 1.346(13) .
C7 H7 0.9300 .
C8 H8 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
C3 N1 N2 C1 -1.6(10) . . . .
C3 N1 N2 Zn1 174.1(6) . . . .
O7 Zn1 N2 C1 -13.2(9) . . . .
O7 Zn1 N2 C1 166.8(9) 2_666 . . .
O11 Zn1 N2 C1 76.2(9) . . . .
O11 Zn1 N2 C1 -103.8(9) 2_666 . . .
N2 Zn1 N2 C1 -105(100) 2_666 . . .
O7 Zn1 N2 N1 172.6(6) . . . .
O7 Zn1 N2 N1 -7.4(6) 2_666 . . .
O11 Zn1 N2 N1 -98.0(6) . . . .
O11 Zn1 N2 N1 82.0(6) 2_666 . . .
N2 Zn1 N2 N1 81(100) 2_666 . . .
O8 Mo2 O1 Mo3 18.5(7) . . . .
O7 Mo2 O1 Mo3 -86.1(7) . . . .
O5 Mo2 O1 Mo3 161.5(5) 2_667 . . .
O2 Mo2 O1 Mo3 108.9(6) 2_667 . . .
O2 Mo2 O1 Mo3 -177.8(7) . . . .
O8 Mo2 O1 Mo1 -175.4(3) . . . .
O7 Mo2 O1 Mo1 80.0(3) . . . .
O5 Mo2 O1 Mo1 -32.5(8) 2_667 . . .
O2 Mo2 O1 Mo1 -85.0(2) 2_667 . . .
O2 Mo2 O1 Mo1 -11.7(2) . . . .
O10 Mo3 O1 Mo2 -11.5(7) . . . .
O9 Mo3 O1 Mo2 92.9(7) . . . .
O5 Mo3 O1 Mo2 -130.6(7) 2_567 . . .
O3 Mo3 O1 Mo2 -176.6(7) . . . .
O3 Mo3 O1 Mo2 -102.6(6) 2_567 . . .
O10 Mo3 O1 Mo1 -177.8(3) . . . .
O9 Mo3 O1 Mo1 -73.4(3) . . . .
O5 Mo3 O1 Mo1 63.1(7) 2_567 . . .
O3 Mo3 O1 Mo1 17.1(2) . . . .
O3 Mo3 O1 Mo1 91.1(2) 2_567 . . .
O6 Mo1 O1 Mo2 88.1(8) . . . .
O4 Mo1 O1 Mo2 -88.0(3) . . . .
O3 Mo1 O1 Mo2 167.1(3) . . . .
O2 Mo1 O1 Mo2 13.3(2) . . . .
O5 Mo1 O1 Mo2 89.1(3) . . . .
O6 Mo1 O1 Mo3 -98.8(8) . . . .
O4 Mo1 O1 Mo3 85.1(3) . . . .
O3 Mo1 O1 Mo3 -19.8(2) . . . .
O2 Mo1 O1 Mo3 -173.5(3) . . . .
O5 Mo1 O1 Mo3 -97.8(2) . . . .
O6 Mo1 O2 Mo2 -64.9(3) . . . 2_667
O4 Mo1 O2 Mo2 -172.8(3) . . . 2_667
O3 Mo1 O2 Mo2 60.7(4) . . . 2_667
O1 Mo1 O2 Mo2 99.3(3) . . . 2_667
O5 Mo1 O2 Mo2 18.0(2) . . . 2_667
O6 Mo1 O2 Mo2 -175.6(2) . . . .
O4 Mo1 O2 Mo2 76.6(3) . . . .
O3 Mo1 O2 Mo2 -49.9(4) . . . .
O1 Mo1 O2 Mo2 -11.3(2) . . . .
O5 Mo1 O2 Mo2 -92.7(3) . . . .
O8 Mo2 O2 Mo1 73.5(8) . . . .
O7 Mo2 O2 Mo1 -83.7(3) . . . .
O1 Mo2 O2 Mo1 13.2(2) . . . .
O5 Mo2 O2 Mo1 -174.2(2) 2_667 . . .
O2 Mo2 O2 Mo1 110.9(3) 2_667 . . .
O8 Mo2 O2 Mo2 -37.5(8) . . . 2_667
O7 Mo2 O2 Mo2 165.4(2) . . . 2_667
O1 Mo2 O2 Mo2 -97.7(3) . . . 2_667
O5 Mo2 O2 Mo2 74.9(2) 2_667 . . 2_667
O2 Mo2 O2 Mo2 0.0 2_667 . . 2_667
O6 Mo1 O3 Mo3 -178.1(2) . . . .
O4 Mo1 O3 Mo3 -68.9(3) . . . .
O2 Mo1 O3 Mo3 56.5(4) . . . .
O1 Mo1 O3 Mo3 18.0(2) . . . .
O5 Mo1 O3 Mo3 98.6(3) . . . .
O6 Mo1 O3 Mo3 69.6(3) . . . 2_567
O4 Mo1 O3 Mo3 178.8(2) . . . 2_567
O2 Mo1 O3 Mo3 -55.8(4) . . . 2_567
O1 Mo1 O3 Mo3 -94.3(2) . . . 2_567
O5 Mo1 O3 Mo3 -13.7(2) . . . 2_567
O10 Mo3 O3 Mo1 -65.3(7) . . . .
O9 Mo3 O3 Mo1 77.8(3) . . . .
O5 Mo3 O3 Mo1 175.9(2) 2_567 . . .
O1 Mo3 O3 Mo1 -20.5(2) . . . .
O3 Mo3 O3 Mo1 -110.2(3) 2_567 . . .
O10 Mo3 O3 Mo3 44.9(7) . . . 2_567
O9 Mo3 O3 Mo3 -172.0(2) . . . 2_567
O5 Mo3 O3 Mo3 -73.9(2) 2_567 . . 2_567
O1 Mo3 O3 Mo3 89.7(2) . . . 2_567
O3 Mo3 O3 Mo3 0.0 2_567 . . 2_567
O6 Mo1 O5 Mo3 -88.7(3) . . . 2_567
O4 Mo1 O5 Mo3 106.0(11) . . . 2_567
O3 Mo1 O5 Mo3 15.8(2) . . . 2_567
O2 Mo1 O5 Mo3 167.3(3) . . . 2_567
O1 Mo1 O5 Mo3 91.6(3) . . . 2_567
O6 Mo1 O5 Mo2 84.9(3) . . . 2_667
O4 Mo1 O5 Mo2 -80.4(12) . . . 2_667
O3 Mo1 O5 Mo2 -170.6(3) . . . 2_667
O2 Mo1 O5 Mo2 -19.1(2) . . . 2_667
O1 Mo1 O5 Mo2 -94.8(2) . . . 2_667
O8 Mo2 O7 Zn1 -29.3(13) . . . .
O1 Mo2 O7 Zn1 68.9(13) . . . .
O5 Mo2 O7 Zn1 -130.6(13) 2_667 . . .
O2 Mo2 O7 Zn1 -166.2(9) 2_667 . . .
O2 Mo2 O7 Zn1 143.3(13) . . . .
O7 Zn1 O7 Mo2 128(100) 2_666 . . .
O11 Zn1 O7 Mo2 -78.6(13) . . . .
O11 Zn1 O7 Mo2 101.4(13) 2_666 . . .
N2 Zn1 O7 Mo2 -169.6(13) 2_666 . . .
N2 Zn1 O7 Mo2 10.4(13) . . . .
N1 N2 C1 C2 2.1(11) . . . .
Zn1 N2 C1 C2 -172.8(7) . . . .
N2 C1 C2 C3 -1.9(12) . . . .
C1 C2 C3 N1 0.8(10) . . . .
C1 C2 C3 C6 178.3(9) . . . .
N2 N1 C3 C2 0.4(10) . . . .
N2 N1 C3 C6 -177.3(7) . . . .
C8 N3 C4 C5 0.6(13) . . . .
N3 C4 C5 C6 -0.3(14) . . . .
C4 C5 C6 C7 -1.4(13) . . . .
C4 C5 C6 C3 179.8(8) . . . .
C2 C3 C6 C5 176.6(10) . . . .
N1 C3 C6 C5 -6.2(14) . . . .
C2 C3 C6 C7 -2.1(15) . . . .
N1 C3 C6 C7 175.0(8) . . . .
C5 C6 C7 C8 2.7(14) . . . .
C3 C6 C7 C8 -178.5(9) . . . .
C4 N3 C8 C7 0.7(15) . . . .
C6 C7 C8 N3 -2.4(16) . . . .
